Fused Glass Decal Instructions:
Choosing the right decal for your needs;
Fused glass decals come in low-fire and high-fire.
First determine which product you are purchasing so that you will know which schedule to use for these glass fusing decals.
Low-fire decals are generally fired to between 1034-1074 degrees Fahrenheit,
High-fire decals go up to temperatures between 1280-1320 degrees Fahrenheit.
Prepared kiln shelf
1. Determine which glass you want as your background and fuse two or more pieces together to a full fuse to achieve a smooth piece.
2. Cut the decal to the desired shape and size.
3. Cleanse glass with desired glass cleaner. Dry the piece with a lint free towel.
4. Remove sheet of paper that is protecting the decal.
5. Pour distilled water into clean container.
6. Soak pre-cut decal in water until it can be easily slid off of background paper.
7. Slowly and delicately slide decal onto glass.
8. Blot decal with paper towel removing any unwanted bubbles from under decal.
9. Allow piece to dry thoroughly. All the moisture must be removed from the piece before firing in kiln. This may take up to 24 hours. Dry for a minimum of 12 hours.
10. Place piece on kiln shelf that has been either washed with kiln wash or protected with kiln paper.
11. Shut the lid or access. Use kiln posts to vent kiln about 1-2 inches. The posts should be placed so that the kiln lid is open about 1-2 inches to vent the kiln and allow the materials from the medium to burn off.
12. Start the kiln.
13. Heat kiln at approximately 250 degrees per hour to 350 degrees Fahrenheit and hold at this temperature for 20 minutes.
14. Heat kiln at around 500 degrees per hour to 1000 degrees Fahrenheit.
15. Soak piece for about 10 minutes to allow the glass to even out in temperature.
16. Take piece up as fast as possible to final firing temperature. This would be 1034-1074 degrees Fahrenheit for low fire decals and 1280-1320 for high fire decals.
17. Soak at this temperature for 8-10 minutes.
18. Bring piece down to annealing temperature (900 degrees Fahrenheit for Bullseye Glass) and hold for 1 hour.
19. Turn off and unplug the unit. If the unit is built with heavy fire bricks, you can allow it to cool off by itself. On the other hand if it is assembled with ceramic fiber, the unit must be kept on and monitored so that it does not cool down more than about 300 degrees Fahrenheit per hour.
20. When the temperature drops beneath 100 degrees Fahrenheit, the kiln may be opened.
Decals go on your FINISHED, fire polished piece.
DO NOT cap the decals with a top glass layer.
Decal firing is the last step to your piece.